1. ELEMENTS OF MAGNETISM
where Ndis is the average number of displacement generated by each ion, Ns is the atomic surface density of the material, is the ion dose and a lattice parameter. For example, Ga ion implantation, by focused ion beam, leads to the reduction of exchange coupling between magnetic grains and the formation of extended domain wall pinning defects in Co film. These e↵ects lead to a square hysteresis loops and a dramatic in-crease in coercivity (as shown in ). On the other hand, a Ga+ dose of 1014 ions / cm2 induces a complete transition from the ordered L10 to the disordered A1 phase in FePt thin film, leading to a drastic decrease of the magnetic anisotropy and coercivity, and to a spin reorientation transition from out-of-plane to in-plane .
Ion irradiation is revealed to be a very flexible tool to tailor the main magnetic prop-erties (e.g., anisotropy, coercive field, exchange interaction, Curie temperature) of thin films and multilayers, giving rise to several e↵ects, depending on the chosen parameters, like intermixing, modification of morphology, interface quality and strain, modification of crystallinity and chemical composition, production of vacancies and pinning centers [29, 30, 31, 32].
1.6 The exchange-spring system
were highlighted, regarding both the crystallographic alignment and the control of suf-ficiently small soft regions, to avoid the easy nucleation of reversed domains.
A similar material has been also suitably structured at the nanometer scale, such as coupled bilayer films, providing convenient model systems for studying the magnetic properties of the exchange system because the relative length scales (i.e., thicknesses of the hard- and soft-magnet layers) can be controlled during the deposition process. The hard/soft multilayer becames a model system to study and understand the properties of exchange-spring systems, but on the other hand also promising candidate for the de-sign of thin-film permanent magnets. Nowadays, it could found possible applications as micro-electro-mechanical devices (MEMS) where thin-film permanent magnets can be employed in high-quality and performance integrated micro-actuators, micro-motors or micro-pumps and in recent years they are proposed as perpendicular recording media .
Many theoretical approaches have been considered in order to explain the magnetiza-tion reversal process in exchange coupled bilayers. In particular, they can be classified as:
• Model base on micromagnetic calculations with continuum as well as discrete approach leading to analytic expressions of the relevant parameters [35, 36, 37, 38, 39, 40]
• Computational approaches by solving the dynamic equation of motion 
• First principle calculation of the band-energy structure 
These models assume the in-plane orientation of the magnetization and a common re-sult was the definition of the soft phase thickness (ds) as an important parameter in determining the magnetization reversal process and thus the shape of the hysteresis loop, besides the exchange length of the hard phase (lw,h=p
Ah/Kh). Asti et al. 
developed a model based on a multilayer composed of hard and soft layers of finite thickness. By studying the sign of c, calculated at the critical field corresponding to the start of flux reversal, as a function of the half-thickness of the hard (th) and soft (ts) layers, a magnetic phase diagram for the planar hard/soft multilayer was obtained (Fig. 1.19 (b)).
Increasing the thickness of the hard or soft layers three regimes have been obtained:
1. ELEMENTS OF MAGNETISM
Figure 1.13: a) reversible spin rotation in the soft layer; b) magnetic phase diagram calculated in  for a Fe/NdFeB bilayer, t1and t2are the half thicknesses of the soft and hard layer, respectively
the previous model. The position of the critical curves between the regimes is determined by intrinsic (K, MSand A) and extrinsic parameters of the multilayer (th, ts). The rigid magnet regime corresponds to the highest maximum energy product, with values of 75 MGOe for Fe(8 nm)/SmCo(3 nm) and 100 MGOe for Fe(4.4 nm)/NdFeB(1.8 nm) bilayers, due to a square hysteresis loop with a unique value of the critical field. As to the exchange-spring regime, its existence also depends on the ratio between the anisotropy constants of the two phases: for soft/SmCo the ES region disappears when Ks/Kh 0.06. Thus, a requirement can be deduced for the existence of the exchange-spring system: the anisotropy of the soft phase has to be less than few percent of the hard phase anisotropy. A further increase in Ks/Khleads to the disappearance of the decoupled regime, too. The two phases are now too similar to give an independent contribution and only the RM regime exists.
In , the results of the model are compared with previous theoretical ap-proaches and experimental works. The limit of the hard bulk with a soft planar inclusion is considered and compared with previous models, e.g. . The com-parison with discrete micromagnetic models employed to reproduce the experi-mental hysteresis loops [32, 31] or to investigate the effect of nanostructuration  is made. The agreement is good down to thicknesses of few atomic layers, where the discrete micromagnetic approach results to be more reliable. With this kind of approach, Amato et al.  demonstrated that on increasing nanostruc-turation, i.e. increasing the number of layers while keeping constant the total thickness and the hard/soft ratio, both the coercivity and the total thickness are
Figure 1.19: - a) reversible rotation of the magnetic moments in the soft layer. b) Magnetic phase diagram for a Fe/NdFeB bilayer, in terms of soft (t1) and hard (t2) layer thicknesses
the rigid composite magnet (RM), the exchange-spring magnet (ES) and the decoupled magnet (DM). Each with similar characteristics compared to the results of the previous model. The position of critical curves between the regimes is determined by intrinsic (K, MS and A) and extrinsic parameters of the multilayer (th, ts). In the rigid magnet regime the highest maximum energy product is achieved, with values of 75 MGOe for Fe(8 nm)/SmCo(3 nm) and 100 MGOe for Fe(4.4 nm)/NdFeB(1.8 nm) bilayers, due to a square hysteresis loop with a unique value of the critical field. The existence of the exchange-spring regime also depends on the ratio between the anisotropy constants of the two phases: for soft/SmCo the ES region disappears when Ks/Kh 0.06. Thus to have a ES regime, the anisotropy of the soft phase has to be less than few percent of the hard phase anisotropy. A further increase in Ks/Kh leads to the disappearance of the decoupled regime. The two phases begin too similar to give an independent contribution and only the RM regime remains.
The results of this model have been compared with previous theoretical approaches and experimental works founding a good agreement.
Finally, Asti et al. suggest a possible extension of their model to a system with per-pendicular orientation of the magnetic moments by adding to the total magnetic free energy a shape-anisotropy term of the form 2⇡MS2, obtaining the magnetic phase diagram in figure 1.20. In this model di↵erent assumptions have been made:
• The infinite exchange-spring multilayer is supposed to be made of alternate soft and hard layers perpendicular to the x-axis.
1.6 The exchange-spring system
with a detailed description of the magnetization reversal pro-cess, in the case of planar-anisotropy systems2,3
!easy mag-netization direction in the film plane ". In the present work we will discuss an extension of our model to include the case of a hard phase with perpendicular anisotropy. Applying a mag-netic field perpendicular to the film plane, a nonuniform magnetization distribution results due to the competition be-tween the perpendicular anisotropy of the hard phase and the in-plane shape anisotropy of both phases. This particular dis-tribution !named perpendicular exchange spring"14
drives the switching process of the whole system. A crucial point in this subject concerns the demonstration, made in the present work, of the validity of the one-dimensional assumption for the perpendicular situation. The model has also been applied to the case of external magnetic field parallel to the film plane.
In order to verify the predictions of the model, we real-ized a series of Fe/FePt bilayers with perpendicular orienta-tion of the hard phase and layers thickness in the range of a few nanometers.
A complete magnetic phase diagram of the Fe/FePt sys-tem is obtained and the dependence of the nucleation field on the layer thickness is calculated and compared to the experi-mental results. Complete hysteresis loops are also achieved by numerical calculations. The theoretical treatment is also extended considering the effect of a reduced interlayer ex-change coupling with respect to the strong coupling assump-tion previously adopted. To this purpose we follow the same representation for the interlayer exchange coupling intro-duced by Guslienko et al.14
and Garcia-Sanchez et al.15
However we admit in our model a nonuniform magnetization distribution of the hard layer and finite magnetocrystalline anisotropy for the soft phase. Our results are acquired en-tirely on the basis of numerical evaluation of the obtained analytical expressions. A comparison is made with the model of Guslienko et al.14
through the application to the FeRh/FePt bilayer system.
The paper is organized as follows. A description of the adopted micromagnetic model for the cases of perpendicular anisotropy and strong interlayer coupling is the content of Sec. II A. The effect of a reduced interlayer coupling is ana-lyzed in Sec. II B. Section III reports the application of the
retical predictions are exposed in Sec. IV. Finally the appli-cation of the model to the FeRh/FePt bilayer is considered in Sec. V.
II. THE MICROMAGNETIC MODEL
Hereafter we will describe the mathematical procedure utilized in our micromagnetic analysis for perpendicular magnetic anisotropy, with the field applied perpendicular to the film plane, for the cases of strong and reduced interlayer exchange coupling. The model is based on the continuum approximation and this implies that it should become inad-equate when the layer thicknesses are comparable with the interatomic distance.3
However, the comparison with the re-sults of discrete one-dimensional models for the case of pla-nar anisotropy13
shows that the micromagnetic approach well represents the real system, down to thickness of a few atomic layers.
A. The case of strong interlayer exchange coupling
In the adopted model the following assumptions have been made:
1. The !infinite" exchange-spring multilayer is supposed to be made of alternate soft and hard layers perpendicular to the x axis !see the scheme in Fig. 1".
2. The two component layers are assumed to have uniaxial anisotropy with symmetry axes both perpendicular to the film plane, along the x axis !Fig. 1".
3. Only periodical solutions are considered, so that the median planes of the layers are symmetry planes for the magnetic structure.
4. The magnetization is uniform on each plane of the system, that is, no magnetic domains are present in the film plane.
5. The magnetization Mi
in both hard and soft layers stay in the xz plane and the angles !i
represent the orientation angle of Mi
with respect to the x axis. This implies that theFIG. 1. Basic scheme for the one-dimensional continuum
micro-magnetic model of the hard/soft multilayer with anisotropy-axis perpendicular to the film plane.
FIG. 2. Magnetic phase diagram in the plane of layer thick-nesses t1 !soft" and t2 !hard" for a Fe/FePt bilayer with perpendicu-lar anisotropy and the parameters reported in Sec. III. The figure reports the critical "# line !"c!#, full line" together with the isofield line corresponding to Hc1=0!dashed line". RM=rigid mag-net; ES=exchange-spring magnet.
ASTI et al. PHYSICAL REVIEW B 73, 094406 !2006"
Figure 1.20: - Magnetic phase diagram in the plane of layer thickness t1soft and t2hard for a Fe/FePt bilayer with perpendicular anisotropy. After .
• The two component layers are assumed to have uniaxial anisotropy with symme-try axes both perpendicular to the film plane.
• Only periodical solutions are considered.
• No magnetic domains are present in the film plane.
• The problem has a one-dimensional character.
• A strong interlayer exchange coupling is considered.
An analytical solution for free energy density has been given:
( 1)i Z xi
FidxFi= Ai[( #
x)2] + µ0MiHcos# + Lisin2# (1.52) where represents the angle between the projection of magnetization in the y-z plane and the z axis, L is the total anisotropy constants and i=1,2.
One open issue for all theoretical model remain to estimate the thermal stability and energy barrier of the exchange system respect with other system. A simple analytical model for the optimization of a single phase data layer is given when assuming that the film is composed of weakly coupled single domain grains . In this case the energy barrier for a single domain particle is given by
E = KV (1 H
1. ELEMENTS OF MAGNETISM
where V is the volume of the grain and H is the e↵ective field acting on the grain parallel to the easy axis. K is the e↵ective anisotropy, which is the sum of the uniaxial anisotropy K1 and the shape anisotropy. The exchange field among the neighboring grains stabilizes the grain, opposing the demagnetizing field. The e↵ective field can be written, in MKS international units system, as:
H = Js µ0
(1.54) Assuming all grains except one to be reversed, the switching field of the last grain, called saturation field or closer field, can be expressed as
HSW = 2K
Js Bexµ0+ Js
By setting the first derivative of Eq. 1.53 with respect to K at zero, the values for K and Js that maximize the energy barrier for a given field can be obtained .
K = 1
32µ0(3Bh+ 3Bex )(Bh+ Bex+ ) (1.56) with =q
5Bh2+ 6BhBex+ B2ex . Considering Js = 1/4(3Bh+ 3Bex ) the energy barrier can be expressed as
E(Bh, Bex) = V(3Bh+ 3Bex )( Bh+ Bex+ )2
8µ0(Bh+ Bex+ ) (1.57)
figure 1.21 shows the calculated energy barrier as a function of Js Exchange coupled
total thickness!f =!hard/!total" on the energy barrier, where f=1 describes a medium consisting of one complete hard magnetic layer. An exchange field of 0.2 T was assumed in the calculation. This is about 12% of the coercive field. First, both layers are set to an identical saturation polarisation!Js
=Js,hard=Js,soft". Figure 2 shows the calculated energy barrier as a function of f. Under the constrain of a saturation field of 1.7 T, the highest-energy barrier is obtained for f =0.375 and for Js=0.5 T. The energy barrier of this optimal bilayer is more than two times larger than that of the single phase medium. The influence of Json the energy barrier for differ-ent film architectures is given in Fig. 3. For a single layer, the finite element simulations results in an energy barriers with a maximum at Js=0.42 T, in excellent agreement with the ana-lytic model predicting Js=0.41 T.
As a second step, different values of Jsfor the hard and soft layer are used. The optimal bilayer is found for the mag-netic properties listed in the caption Fig. 1!a". The energy barrier increases to 48 kBT300—compared to 19 kBT300 for the optimum single phase media. The influence of an
ex-change breaking layer between the soft and the hard layer on the energy barrier was investigated for Js,hard=Js,soft=0.5 T for different values of the fraction f. In a 1 nm thick spacer layer separating the hard and soft layer, the exchange con-stant was reduced by a factor of 2, 3, 4, 5, and 6. The results show that for all those values, the energy barrier decreases.
A small angular dependence of the coercive field is im-portant in order to obtain a high signal to noise ratio.11For the composite media, the angular dependence of the coercive field can be fitted with the expression Hc!!"=Hc!0"/cos!!".
This expression is commonly used for magnetic materials which are controlled by domain-wall pinning. For an angle! between 0° and 40°, the deviation of the analytic formula and the finite element calculation are less than 5%. In contrast to exchange spring media, single phase media exhibit a strong angular dependence of the coercive field!described by the SW theory". For a misalignment of 10° between the external field and the easy axis, the coercive field increases by a fac-tor of 1.01 for the composite media, whereas it decreases by a factor of 0.68 for the single phase media.
In conclusion, it was shown that exchange spring media can improve thermal stability by a factor of 2 compared to single phase media allowing at constant coercivity. The dif-ferent magnetization state during switching in the head field compared to thermal switching allows one to optimize ther-mal stability and coercivity mostly independent from each other, resulting in a significant reduction of the stable grain size. Recent experiments by Okamoto et al.12showed that these properties indeed can be optimized independently.
They prepared epitaxial FePt L10nanoparticles covered with different Pt overlayer thicknesses. They observe a decrease of coercivity with Pt thicknes while the energy barrier re-mains unaltered. These experiments can be explained by an induced magnetization within the Pt layer resulting in a kind of exchange coupled bilayer—in qualitative agreement with the exchange spring media described in this letter.
The financial support of the Austrian Science Fund Grant No. Y-132-N02 is acknowledged.
1Y. Kanai, R. Matsubara, H. Watanabe, H. Muraoka, and Y. Nakamura, IEEE Trans. Magn. 39, 1955!2003".
2N. A. Usov, C. Chang, and Z. Wei, Appl. Phys. Lett. 83, 3749!2003".
3S. Cumpson, P. Hidding, and R. Coehoorn, IEEE Trans. Magn. 36, 2271
!2000"; J. J. M. Ruigrok, R. Coehoorn, S. R. Cumpson, and H. W. Kes-teren, J. Appl. Phys. 87, 5298!2000".
4J. U. Thiele, S. Maat, and E. Fullerton, Appl. Phys. Lett. 82, 2859!2003".
5R. H. Victora and X. Shen, IEEE Trans. Magn. 41, 537!2005".
6D. Suess, T. Schrefl, R. Dittrich, M. Kirschner, F. Dorfbauer, G. Hrkac, and J. Fidler, J. Magn. Magn. Mater. 290, 551!2005".
7E. F. Kneller and R. Hawig, IEEE Trans. Magn. 27, 3588!1991".
8E. Fullerton, J. Jiang, M. Grimsditch, C. Sowers, and S. Bader, Phys. Rev.
B 58, 12193!1998".
9D.-X. Chen, J. A. Brug, and R. B. Goldfarb, IEEE Trans. Magn. 27, 3601
10R. Dittrich, T. Schrefl, D. Suess, W. Scholz, H. Forster, and J. Fidler, J.
Magn. Magn. Mater. 250, 12!2002".
11K. Z. Gao and N. Bertram, IEEE Trans. Magn. 38, 3675!2002".
12S. Okamoto, O. Kitakami, N. Kikuchi, T. Miyazaki, Y. Shimada, and T.
Chiang., J. Phys.: Condens. Matter 16, 2109!2004".
FIG. 2. Energy barrier as a function of the fraction of the hard layer thick-ness to the total thickthick-ness for a magnetic bilayer structure. Different curves are for different magnetic polarization which are set to be the identical for the hard magnetic and soft magnetic layer.
FIG. 3. Energy barrier as a function of Jsfor the single layer and the bilayer.
In the bilayer, the same value of Jsis taken in the hard and soft part.
012504-3 Suess et al. Appl. Phys. Lett.87, 012504 !2005"
Downloaded 04 Jul 2011 to 220.127.116.11. Redistribution subject to AIP license or copyright; see http://apl.aip.org/about/rights_and_permissions
Figure 1.21: - Energy barrier as a function of Jsfor the single layer and the bilayer. In the bilayer, the same value of Jsis taken in the hard and soft part.
composite (ECC) media, based on exchange-spring system, has been shown to possess
1.6 The exchange-spring system
several major advantages relative to conventional perpendicular media, including a reduction in the switching field of approximately a factor two for the same thermal stability and stronger magnetic anisotropy energy. In particular, there is a ratio between the thermal barrier of the media and its switching field, which can be defined as 
⇠ = 2 E
where Hs, Ms, V are the switching field, the saturation magnetization and magnetic volume, respectively. For this ECC media, this ratio ⇠ approach two, making ECC media quite promising for ultra high-density recording (see paragraph 1.7.1). A related advantage is that ECC media allowing a much higher track density for a given writer than a conventional media .
1.6.1 Graded exchange spring system
The idea of exchange spring media with varying anisotropies in each layer was fur-ther extended by changing the anisotropy gradually from two to N layers, approaching towards a graded media system. Following the results obtained by Suess  in this system, the coercive field of the multilayer structure was found to decrease with 1/N while the energy barrier was only determined by the magnetic properties of the hardest layer (Fig. 1.22). A drastic reduction of Hpinning, the field at which completely magne-tization reverse occurs, can be realized if the anisotropy constant depends quadratically with the thickness (x), such as K(x) = ↵x2 = x2Khard/t2Gwith tG is the total thickness of the grain. The media has its maximum anisotropy constant corresponding to the top of the grain (Khard) and the pinning field follows
Hpinning = (2/Js)p
Suess shown that the energy barrier in graded media linearly decreases with the mag-netic field . This result demonstrates that the energy barrier of graded media is further enhanced relative to the single phase barrier because of this unexpected linear field dependence, resulting in even higher thermal stability. The field dependence of the energy barrier Eb(H) is determined and found to be linear . A simple explana-tion is provided for this linear dependence on the basis of the magnetizaexplana-tion reversal
1. ELEMENTS OF MAGNETISM
sumption of the analytically calculated pinning field is ful-filled!large tG", Eq. !3" excellently agrees with the numerical calculation. If instead of a quadratic change of the aniso-tropy, K1is increased linearly as a function of x the coercive field drastically increases to 2.0 T. Figure 2 shows the reduc-tion of the coercive field of a hard magnetic layer with a thickness of 20 nm and an anisotropy constant Khardthat is coupled to a G layer with thickness tGand a maximum an-isotropy of Khard. The coercivity reduction is calculated for different structures with different Khardvalues. The coercivity reduction r=Hpinning/Hc,hard can also be calculated analytically using Eq. !3" For the reduction it follows r=!1/tG"#A/Khard.
Finally, it will be shown that the introduction of soft layers in principle does not influence the thermal stability at zero external field. The energy barrier of a single phase me-dia !material parameters are given in Fig. 1" is compared with the energy barrier of the trilayer of Fig. 1. The energy barrier is calculated using the nudged elastic band method.14 Figure 3 shows that thermal fluctuations may form a nucle-ation at the end of the particle. This nuclenucle-ation propagates through the particle. For the single phase media the formed domain wall has largest energy when it is located exactly in the center of the grain. The energy barrier is equal to the domain wall energy in the hard region!for a cylindrical grain with diameter of 5 nm !E=84kBT300". Interestingly the situ-ation is very similar for the trilayer structure. Again a domain wall is formed at the bottom of the grain. The energy of the domain wall successively increases as it is driven by thermal fluctuations in the harder layers. The domain wall has largest energy, when it is located in the hardest layer. Since the hardest layer has the same material properties as the single grain the domain wall energies are the same. Due to the finite layer thickness of 7 nm of the hardest layer in the trilayer, not a full domain wall is formed, leading to a reduction of the energy barrier of about 7%. The energy barrier of G layer with thickness of 25 nm is about 30% smaller than that of the single layer. However, the energy barrier can be in-creased by coupling the G layer to a hard magnetic layer with constant anisotropy and matching the values of the
anisotropies at the interface. The thermal stability is only determined by the magnetic properties in the hardest mag-netic layer.
In conclusion it was shown that an optimal design of a magnetic bilayer structure for recording media requires a hard magnetic layer with properties similar to state of the art perpendicular recording media. This hard layer is coupled to a second layer that has in the optimal case an anisotropy that is about five times larger. Most important it was demon-strated that the energy barrier in multilayer exchange spring media is not proportional to the coercive field. The coercive filed is proportional to 1 over the number of layers while the energy barrier is constant.
The author is very grateful for great discussion with T. Schrefl and J. Fidler.
1D. Weller, A. Moser, L. Folks, M. E. Best, W. Lee, M. F. Toney, M.
Schwickert, J. U. Thiele, and M. F. Doerner, IEEE Trans. Magn. 36, 10
2C. Lim, E. Kim, Y. Kim, and H. Oh, Intermag, San Diego!2006" Paper No. DR04.
3J. J. Miles, D. M. McKirdy, R. W. Chantrell, and R. Wood, IEEE Trans.
Magn. 39, 1876!2003".
4R. H. Victora and X. Shen, IEEE Trans. Magn. 41, 2828!2005".
5D. Suess, T. Schrefl, S. Fahler, M. Kirschner, G. Hrkac, F. Dorfbauer, and J. Fidler, Appl. Phys. Lett. 87, 012504!2005".
6J. P. Wang, W. K. Shen, and J. M. Bai, IEEE Trans. Magn. 41, 3181
7H. Kronmüller and H. R. Hilzinger, J. Magn. Magn. Mater. 154, 3!1976".
8K. Y. Guslienko, O. Chubykalo-Fesenko, O. Mryasov, R. Chantrell, and D. Weller, Phys. Rev. B 70, 104405!2004".
9F. B. Hagedorn, J. Appl. Phys. 41, 2491!1970".
10H. Kronmuller and D. Goll, Physica B 319, 122!2002".
11D. Suess, J. Magn. Magn. Mater..
12A. Dobin and H. J. Richter, e-print cond-mat/0605368.
13J. S. Jiang, J. E. Pearson, Z. Y. Liu, B. Kabius, S. Trasobares, D. J. Miller, S. D. Bader, D. R. Lee, D. Haskel, G. Srajer, and J. P. Liu, J. Appl. Phys.
14R. Dittrich, T. Schrefl, D. Suess, W. Scholz, H. Forster, and J. Fidler, J. Magn. Magn. Mater. 250, 12!2002".
FIG. 2. Reduction of the coercive field if a layer with gradually increasing anistropy of thickness tgand a maximum anisotropy of Khardis fully ex-change coupled to a hard magnetic layer. The value of the anistropy constant Khardof the hard layer is changed from 1 to 4 MJ/m3.
FIG. 3. Energy barrier and thermally activated switching process for a single phase media and the trilayer of Fig. 1. The hardest layer of the trilayer is 7 nm. The grain diameter is 5 nm. The z component of the magnetization during thermally activated switching is color coded.
113105-3 D. Suess Appl. Phys. Lett.89, 113105 !2006"
Downloaded 05 Jul 2011 to 18.104.22.168. Redistribution subject to AIP license or copyright; see http://apl.aip.org/about/rights_and_permissions
Figure 1.22: - Energy barrier and thermally activated switching process for di↵erent exchange systems calculated by Suess .
mechanism of graded media, which is not a rigid rotation, but proceeds via domain walls motion. Energy barrier dependance can be calculated as
Eb(H) = 4p
AK (2tG p
taking into account two energy terms such as the energy of the domain wall formation and the di↵erence of the Zeeman energies between the up and the down spin regions.
In general in graded media, the reversal pathways of magnetization reversal proceeds via a partial domain wall that gradually pass through the whole thickness, instead of an avalanche-like runaway reversal, which is theorize for homogeneous phase media.
This makes graded media more suitable for magneto recording application than other multilayer system.